# Photophysical Properties of Multilayer Graphene–Quantum Dots Hybrid Structures

^{1}

^{2}

^{*}

## Abstract

**:**

^{8}s

^{−1}strongly inhibits photoinduced processes on the QD surfaces and provides photostability for QD-based structures.

## 1. Introduction

_{2}and graphene [21,22]. Hybrid systems based on graphene and semiconductor QDs are the most popular solutions for achieving high efficiency in the conversion of absorbed energy into useful signals for the final photoelectric device [23,24,25,26].

^{8}s

^{−1}should strongly inhibit photoinduced processes on the QDs’ surfaces and provide photostability for QD-based structures.

## 2. Materials and Methods

#### 2.1. Materials

#### 2.2. Ligand Exchange Procedure

#### 2.3. Formation of MLG–QD Hybrid Structures Layered on Slides

#### 2.4. Characterization of the Structures

_{i}is the amplitude of the ith (1st or 2nd) decay component and τ

_{i}is the characteristic decay time of the ith component.

_{smpl}and φ

_{ref}are the quantum yields for QDs and rhodamine 6G luminescence, respectively; I

_{smpl}and I

_{ref}are the intensities at the maxima of the luminescence band for QDs and rhodamine 6G, respectively; D

_{smpl}and D

_{ref}are optical densities at the luminescence excitation wavelength for QDs and rhodamine 6G, respectively; n

_{smpl}and n

_{ref}are the refractive indices of the solvents toluene and ethanol, respectively [40].

## 3. Results and Discussion

#### 3.1. PL Kinetics of CdSe QDs in MLG–QD Structures

_{1}and τ

_{2}, are further referred to as fraction 1 and fraction 2, respectively.

_{ri}and k

_{nri}are radiative and nonradiative rates of exciton deactivation, respectively; τ

_{i}and φ

_{i}are the PL decay time and QY of the 1st and 2nd QD fractions, respectively.

_{ri}= k

_{r}= 4∙10

^{7}s

^{−1}), according to [42]. Therefore, the difference in PL decay time is caused by different nonradiative rates (k

_{nri}) only. In our QD monolayer samples, both QD PL fractions with τ

_{1}~2 ns and τ

_{2}~7 ns give approximately the same contribution to the PL signal. A schematic representation of various radiative and nonradiative relaxation pathways of the excited state in QDs for a MLG–QD hybrid structure system is shown in Figure 2.

_{0}are QD PL intensities after and before interaction with MLG; A

^{i}is the amplitude of the ith QD fraction; τ

^{i}is the PL decay time of the ith QD fraction; τ

_{r}is the radiative time of CdSe QDs, which is equal to 25 ns [32].

_{i}

^{G}) with MLG in the structures, as follows:

_{i}

^{G}is the PL decay time of the ith QD fraction in hybrid structures.

_{i}

^{G}) of their interactions with MLG (Q

_{i}

^{G}referring to Table 2, showing 98% and 97.5% for 1st and 2nd QD fractions, respectively). It should be noted that using Equation (7), we can estimate the minimal rate of QD interaction with MLG that totally quenches the PL of QDs in the hybrid structures, which is no less than 0.4 × 10

^{8}s

^{−1}.

#### 3.2. Photoelectric Properties of MLG–QD Hybrid Structures

_{i}is the amplitude and t

_{i}is the characteristic time for stage I. The fitting parameters of the photoresponses for MLG and hybrid structures are presented in Table 3.

#### 3.3. Photoactivation of MLG–QD Hybrid Structures

^{2}dose showed up to 1.5-fold growth of both the average PL decay time calculated using Equation (2) and the PL intensity. This means that irradiation of QD monolayer samples on dielectric slides by 72 J/cm

^{2}at 405 nm light leads to a decrease in the nonradiative rate in QDs from 6.9 × 10

^{7}s

^{−1}to 2.7 × 10

^{7}s

^{−1}, according to Equations (4) and (5). At the same time, as clearly seen from Figure 4a, there are no changes in the PL decay time or PL intensity of QDs in the MLG–QD hybrid structures. The efficiency of QD photoactivation processes (Q

^{PA}) calculated with Equations (S1) and (S2) clearly decreases by an order of magnitude for QDs located on MLG, in comparison with QDs located on dielectric substrates (i.e., Q

^{PA}of ~100% for QDs on dialectic substrates vs. Q

^{PA}of ~10% for MLG–QDs). This means that the rate of charge or energy transfer from QDs to MLG is much larger than the rate of nonradiative exciton relaxation processes in which trap states are involved. This allows us to estimate the minimal average charge or energy transfer rate from QDs to MLG in our hybrid structures as 〈k

^{G}〉 ≥ 1.0 × 10

^{8}s

^{−1}(according to Table 2). This value demonstrates an excellent agreement with the k

^{G}value estimated for the 1st QD luminescent fraction using PL quenching of QDs in the MLG–QD hybrid structures. This also implies that the k

^{G}value for both QD luminescent fractions is at least 1.0 × 10

^{8}s

^{−1}(see Table 2).

## 4. Conclusions

^{8}s

^{−1}is possible. We show that efficient interaction of QDs with MLG in our MLG–QDs hybrid structures enhances the photoresponse of these structures by a factor of up to 1.5 with respect to MLG. The analysis of the electric properties of the hybrid structures shows that the characteristic photoresponse time of the hybrid structures depends only on the electric properties of MLG and on the architecture of the hybrid structures. We demonstrate for the first time that QD photoactivation in hybrid structures can be an efficient tool for the estimation of the interaction rate of QDs–MLG.

## Supplementary Materials

## Author Contributions

## Funding

## Acknowledgments

## Conflicts of Interest

## References

- Moraitis, P.; Schropp, R.E.; van Sark, W.G.J.H.M. Nanoparticles for luminescent solar concentrators-a review. Opt. Mater.
**2018**, 84, 636–645. [Google Scholar] [CrossRef] - Jeevanandam, J.; Barhoum, A.; Chan, Y.S.; Dufresne, A.; Danquah, M.K. Review on nanoparticles and nanostructured materials: History, sources, toxicity and regulations. Beilstein J. Nanotechnol.
**2018**, 9, 1050–1074. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Jariwala, D.; Sangwan, V.K.; Lauhon, L.J.; Marks, T.J.; Hersam, M.C. Carbon nanomaterials for electronics, optoelectronics, photovoltaics, and sensing. Chem. Soc. Rev.
**2013**, 42, 2824–2860. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Bai, Y.; Mora-Sero, I.; De Angelis, F.; Bisquert, J.; Wang, P. Titanium dioxide nanomaterials for photovoltaic applications. Chem. Rev.
**2014**, 114, 10095–10130. [Google Scholar] [CrossRef] - Chen, G.; Seo, J.; Yang, C.; Prasad, P.N. Nanochemistry and nanomaterials for photovoltaics. Chem. Soc. Rev.
**2013**, 42, 8304–8338. [Google Scholar] [CrossRef] - Pankhurst, Q.A.; Connolly, J.; Jones, S.K.; Dobson, J. Applications of magnetic nanoparticles in biomedicine. J. Phys. D Appl. Phys.
**2003**, 36, 167–181. [Google Scholar] [CrossRef] [Green Version] - Xie, B.; Hu, R.; Luo, X. Quantum dots-converted light-emitting diodes packaging for lighting and display: Status and perspectives. J. Electron. Packag.
**2016**, 138, 020803:1–020803:13. [Google Scholar] [CrossRef] [Green Version] - Carey, G.H.; Abdelhady, A.L.; Ning, Z.; Thon, S.M.; Bakr, O.M.; Sargent, E.H. Colloidal quantum dot solar cells. Chem. Rev.
**2015**, 115, 12732–12763. [Google Scholar] [CrossRef] - Li, X.; Rui, M.; Song, J.; Shen, Z.; Zeng, H. Carbon and graphene quantum dots for optoelectronic and energy devices: A review. Adv. Funct. Mater.
**2015**, 25, 4929–4947. [Google Scholar] [CrossRef] - Dabbousi, B.O.; Rodriguez-Viejo, J.; Mikulec, F.V.; Heine, J.R.; Mattoussi, H.; Ober, R.; Jensen, K.F.; Bawendi, M.G. (CdSe) ZnS core−shell quantum dots: Synthesis and characterization of a size series of highly luminescent nanocrystallites. J. Phys. Chem. B
**1997**, 101, 9463–9475. [Google Scholar] [CrossRef] - Kim, S.; Fisher, B.; Eisler, H.-J.; Bawendi, M. Type-II quantum dots: CdTe/CdSe (core/shell) and CdSe/ZnTe (core/shell) heterostructures. J. Am. Chem. Soc.
**2003**, 125, 11466–11467. [Google Scholar] [CrossRef] - Bera, D.; Qian, L.; Tseng, T.-K.; Holloway, P.H. Quantum dots and their multimodal applications: A review. Materials
**2010**, 3, 2260–2345. [Google Scholar] [CrossRef] [Green Version] - Asryan, L.V.; Suris, R.A. Inhomogeneous line broadening and the threshold current density of a semiconductor quantum dot laser. Semicond. Sci. Tech.
**1996**, 11, 554–567. [Google Scholar] [CrossRef] - Zhang, C.; Palui, G.; Zeng, B.; Zhan, N.; Chen, B.; Mattoussi, H. Non-Invasive Characterization of the Organic Coating of Biocompatible Quantum Dots Using Nuclear Magnetic Resonance Spectroscopy. Chem. Mater.
**2018**, 30, 3454–3466. [Google Scholar] [CrossRef] - Shrestha, A.; Batmunkh, M.; Tricoli, A.; Qiao, S.Z.; Dai, S. Near-Infrared Active Lead Chalcogenide Quantum Dots: Preparation, Post-Synthesis Ligand Exchange, and Applications in Solar Cells. Angew. Chem. Int. Edit.
**2019**, 58, 5202–5224. [Google Scholar] [CrossRef] [PubMed] - Medintz, I.L.; Uyeda, H.T.; Goldman, E.R.; Mattoussi, H. Quantum dot bioconjugates for imaging, labelling and sensing. Nat. Mater.
**2005**, 4, 435–446. [Google Scholar] [CrossRef] - Zhang, H.; Huang, H.; Ming, Y.; Li, H.; Zhang, L.; Liu, Y.; Kang, Z. Carbon quantum dots/Ag
_{3}PO_{4}complex photocatalysts with enhanced photocatalytic activity and stability under visible light. J. Mater. Chem.**2012**, 22, 10501–10506. [Google Scholar] [CrossRef] - Ren, S.; Chang, L.Y.; Lim, S.K.; Zhao, J.; Smith, M.; Zhao, N.; Bulović, V.; Bawendi, M.; Gradecak, S. Inorganic–organic hybrid solar cell: Bridging quantum dots to conjugated polymer nanowires. Nano Lett.
**2011**, 11, 3998–4002. [Google Scholar] [CrossRef] - Biju, V.; Itoh, T.; Abdulaziz, A.; Athiyanathil, S.; Ishikawa, M. Semiconductor quantum dots and metal nanoparticles: Syntheses, optical properties, and biological applications. Anal. Bioanal. Chem.
**2008**, 391, 2469–2495. [Google Scholar] [CrossRef] - De Freitas, J.N.; Grova, I.R.; Akcelrud, L.C.; Arici, E.; Serdar Sariciftcic, N.; Nogueira, A.F. The effects of CdSe incorporation into bulk heterojunction solar cells. J. Mater. Chem.
**2010**, 20, 4845–4853. [Google Scholar] [CrossRef] [Green Version] - Ataca, C.; Şahin, H.; Aktürk, E.; Ciraci, S. Mechanical and electronic properties of MoS2 nanoribbons and their defects. J. Phys. Chem. C
**2011**, 115, 3934–3941. [Google Scholar] [CrossRef] [Green Version] - Ke, Q.; Wang, J. Graphene-based materials for supercapacitor electrodes–A review. J. Materiomics
**2016**, 2, 37–54. [Google Scholar] [CrossRef] [Green Version] - Lin, Y.; Zhang, K.; Chen, W.; Liu, Y.; Geng, Z.; Zeng, J.; Pan, N.; Yan, L.; Wang, X.; Hou, J.G. Dramatically enhanced photoresponse of reduced graphene oxide with linker-free anchored CdSe nanoparticles. ACS Nano
**2010**, 4, 3033–3038. [Google Scholar] [CrossRef] [PubMed] - Xiao, F.X.; Miao, J.; Liu, B. Layer-by-layer self-assembly of CdS quantum dots/graphene nanosheets hybrid films for photoelectrochemical and photocatalytic applications. J. Am. Chem. Soc.
**2014**, 136, 1559–1569. [Google Scholar] [CrossRef] [PubMed] - Fang, Y.; Lv, Y.; Tang, J.; Wu, H.; Jia, D.; Feng, D.; Kong, B.; Wang, Y.; Elzatahry, A.A.; Al-Dahyan, D.; et al. Growth of Single-Layered Two-Dimensional Mesoporous Polymer/Carbon Films by Self-Assembly of Monomicelles at the Interfaces of Various Substrates. Angew. Chem. Int. Edit.
**2015**, 127, 8545–8549. [Google Scholar] [CrossRef] - Chen, W.; Xiao, P.; Chen, H.; Zhang, H.; Zhang, Q.; Chen, Y. Polymeric graphene bulk materials with a 3D cross-linked monolithic graphene network. Adv. Mater.
**2019**, 31, 1802403:1–1802403:15. [Google Scholar] [CrossRef] - Carrillo-Carrión, C.; Cárdenas, S.; Simonet, B.M.; Valcárcela, M. Quantum dots luminescence enhancement due to illumination with UV/Vis light. Chem. Comm.
**2009**, 35, 5214–5226. [Google Scholar] [CrossRef] - Kolesova, E.P.; Maslov, V.G.; Gun’ko, Y.K.; Orlova, A.O. Photoinduced increase of electron transfer efficiency of QDs based hybrid structures. Proc. SPIE
**2019**, 11207, 437–442. [Google Scholar] [CrossRef] - Märker, B.; Hiller, J.; Wackenhut, F.; Braun, K.; Meixner, A.; Scheele, M. Simultaneous positive and negative optical patterning with dye-sensitized CdSe quantum dots. J. Chem. Phys.
**2019**, 151, 141102:1–141102:6. [Google Scholar] [CrossRef] - Cordero, S.R.; Carson, P.J.; Estabrook, R.A.; Strouse, G.F.; Buratto, S.K. Photo-activated luminescence of CdSe quantum dot monolayers. J. Phys. Chem. B
**2000**, 104, 12137–12142. [Google Scholar] [CrossRef] - Pechstedt, K.; Whittle, T.; Baumberg, J.; Melvin, T. Photoluminescence of colloidal CdSe/ZnS quantum dots: The critical effect of water molecules. J. Phys. Chem. C
**2010**, 114, 12069–12077. [Google Scholar] [CrossRef] - Bawendi, M.G.; Carroll, P.J.; Wilson, W.L.; Brus, L.E. Luminescence properties of CdSe quantum crystallites: Resonance between interior and surface localized states. J. Chem. Phys.
**1992**, 96, 946–954. [Google Scholar] [CrossRef] - Gaponik, N.; Talapin, D.V.; Rogach, A.L.; Hoppe, K.; Shevchenko, E.V.; Kornowski, A.; Eychmüller, A.; Weller, H. Thiol-capping of CdTe nanocrystals: An alternative to organometallic synthetic routes. J. Phys. Chem. B
**2002**, 106, 7177–7185. [Google Scholar] [CrossRef] - Bao, H.; Gong, Y.; Li, Z.; Gao, M. Enhancement effect of illumination on the photoluminescence of water-soluble CdTe nanocrystals: Toward highly fluorescent CdTe/CdS core-shell structure. Chem. Mater.
**2004**, 16, 3853–3859. [Google Scholar] [CrossRef] - Reiss, P.; Bleuse, J.; Pron, A. Highly luminescent CdSe/ZnSe core/shell nanocrystals of low size dispersion. Nano Lett.
**2002**, 2, 781–784. [Google Scholar] [CrossRef] - Kannan, P.K.; Moshkalev, S.A.; Rout, C.S. Highly sensitive and selective electrochemical dopamine sensing properties of multilayer graphene nanobelts. Nanotechnology
**2016**, 27, 075504:1–075504:9. [Google Scholar] [CrossRef] - Justo, Y.; Moreels, I.; Lambert, K.; Hens, Z. Langmuir–Blodgett monolayers of colloidal lead chalcogenide quantum dots: Morphology and photoluminescence. Nanotechnology
**2010**, 21, 295606:1–295606:6. [Google Scholar] [CrossRef] - Black, A.; Roberts, J.; Acebrón, M.; Bernardo-Gavito, R.; Alsharif, G.; Urbanos, F.J.; Juárez, B.H.; Kolosov, O.V.; Robinson, B.J.; Miranda, R.; et al. Large-Area Heterostructures from Graphene and Encapsulated Colloidal Quantum Dots via the Langmuir–Blodgett Method. ACS Appl. Mater. Int.
**2018**, 10, 6805–6809. [Google Scholar] [CrossRef] [Green Version] - Peng, X.; Manna, L.; Yang, W.; Wickham, J.; Scher, E.; Kadavanich, A.; Alivisatos, A.P. Shape control of CdSe nanocrystals. Nature
**2000**, 404, 59–61. [Google Scholar] [CrossRef] - Fedorov, A.V.; Kruchinin, S.Y.; Baranov, A.V.; Maslov, V.G.; Orlova, A.O. Energy transfer of electronic photo-excitations in semiconductor quantum dots. In Proceedings of the International Conference Fundamentals of Laser Assisted Micro– & Nanotechnologies (FLAMN-07), St. Petersburg, Russia, 25–28 June 2007; p. 132. [Google Scholar]
- Yuan, G.; Gómez, D.E.; Kirkwood, N.; Boldt, K.; Mulvaney, P. Two mechanisms determine quantum dot blinking. ACS Nano
**2018**, 12, 3397–3405. [Google Scholar] [CrossRef] [Green Version] - Brokmann, X.; Coolen, L.; Dahan, M.; Hermier, J.P. Measurement of the radiative and nonradiative decay rates of single CdSe nanocrystals through a controlled modification of their spontaneous emission. Phys. Rev. Lett.
**2004**, 93, 107403:1–107403:4. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Gromova, Y.A.; Reznik, I.A.; Vovk, I.A.; Rackauskas, S.; Alaferdov, A.V.; Orlova, A.O.; Moshkalev, S.A.; Baranov, A.V.; Fedorov, A.V. Photoinduced conductivity enhancement in quantum dot/multilayer graphene nanostructures. Mater. Res. Soc. Symp. Proc.
**2015**, 1787, 15–19. [Google Scholar] [CrossRef] - Reznik, I.A.; Gromova, Y.A.; Zlatov, A.S.; Baranov, M.A.; Orlova, A.O.; Moshkalev, S.A.; Maslov, V.G.; Baranov, A.V.; Fedorov, A.V. Hybrid structures based on quantum dots and graphene nanobelts. Opt. Spectrosc.
**2017**, 122, 114–119. [Google Scholar] [CrossRef] - Xia, F.; Mueller, T.; Lin, Y.M.; Valdes-Garcia, A.; Avouris, P. Utrafast graphene photodetector. Nat. Nanotech.
**2009**, 4, 839–843. [Google Scholar] [CrossRef] [Green Version] - Gromova, Y.; Alaferdov, A.; Rackauskas, S.; Ermakov, V.; Orlova, A.O.; Maslov, V.; Moshkalev, S.A.; Baranov, A.V.; Fedorov, A.V. Photoinduced electrical response in quantum dots/graphene hybrid structure. J. Appl. Phys.
**2015**, 118, 104305:1–104305:6. [Google Scholar] [CrossRef] - Saha, S.K.; Baskey, M.; Majumdar, D. Graphene quantum sheets: A new material for spintronic applications. Adv. Mater.
**2010**, 22, 5531–5536. [Google Scholar] [CrossRef] - Rogach, A.L.; Franzl, T.; Klar, T.A.; Feldmann, J.; Gaponik, N.; Lesnyak, V.; Shavel, A.; Eychmüller, A.; Rakovich, Y.P.; Donegan, J.F. Aqueous synthesis of thiol-capped CdTe nanocrystals: State-of-the-art. J. Phys. Chem. C
**2007**, 111, 14628–14637. [Google Scholar] [CrossRef] - Farmer, D.B.; Golizadeh-Mojarad, R.; Perebeinos, V.; Lin, Y.-M.; Tulevski, G.S.; Tsang, J.C.; Avouris, P. Chemical doping and electron−hole conduction asymmetry in graphene devices. Nano Lett.
**2009**, 9, 388–392. [Google Scholar] [CrossRef] [Green Version] - Moon, H.; Lee, C.; Lee, W.; Kim, J.; Chae, H. Stability of Quantum Dots, Quantum Dot Films, and Quantum Dot Light-Emitting Diodes for Display Applications. Adv. Mater.
**2019**, 34, 1804294:1–1804294:14. [Google Scholar] [CrossRef]

**Figure 1.**Photoluminescence (PL) decay curves of 5.5 nm CdSe–ZnS quantum dots (QDs) on a dielectric slide (green rectangles) and in the multilayer graphene (MLG)–QD structures (black triangles). A 405 nm pulse laser was used for PL excitation of QDs. Solid lines (green and black) are biexponential fits of the decay. Inset: table showing the fitting parameters of PL decay curves.

**Figure 2.**Schematic representation of radiative and nonradiative pathways of the excited state in QDs.

**Figure 3.**(

**a**) The photoresponse of MLG (black line) and MLG–QD hybrid structures (red line) with irradiation with a 405 nm laser (dashed regions). (

**b**) Enlarged parts of the curves (black and red circles) with biexponential fitting (green and purple line).

**Figure 4.**Photoactivation of QD monolayer and MLG–QD hybrid structures. (

**a**) Irradiation dose dependence of the photoresponse amplitude of MLG–QD structures (blue spots) and of the average PL decay time of QDs layered on dielectric slides (red triangles) and in the hybrid structures (green rectangles). Solid lines are guidelines for the eye. (

**b**) Photoluminescence (PL) spectra of QDs before photoactivation (black rectangles and triangles) and after exposure to 72 J/cm

^{2}of UV light (red circles, green rectangles) on dielectric slides (black rectangles, red circles) and in the hybrid structures (black triangles, green rectangles).

Samples | Characteristics |
---|---|

MLG | Multilayered graphene nanobelts with 30–40 nm thickness deposited on a glass slide with titanium contacts |

QDs | 5.5 nm core–shell CdSe–ZnS QD monolayer deposited on a glass slide from toluene solution |

MLG–QDs | Hybrid structures with 5.5 nm core–shell CdSe–ZnS QD monolayer deposited on the MLG on a glass slide with titanium contacts |

**Table 2.**The photophysical properties of CdSe–ZnS QD monolayers on glass slides and in hybrid structures based on MLG.

Samples | Parameters | Units | 1st QD fraction | 2nd QD fraction | Formula |
---|---|---|---|---|---|

CdSe–ZnS QDs monolayer | k_{r} | s^{−1} | 0.4 × 10^{8} | - | |

φ_{i} | % | 8.4 | 27.7 | (5) | |

τ_{i}^{QD} | ns | 2.1 ± 0.1 | 6.9 ± 0.1 | - | |

A_{i} | Counts | 1350 ± 50 | 1100 ± 50 | - | |

k_{nr} | s^{−1} | 4.3 × 10^{8} | 1.0 × 10^{8} | (4) | |

Hybrid structures | τ_{i}^{G} | ns | 1.2 ± 0.1 | 5.5 ± 0.3 | - |

A_{i} | Counts | 47 ± 2 | 34 ± 2 | - | |

k_{i}^{G} | s^{−1} | (3.4 ± 0.2) × 10^{8} | (0.40 ± 0.05) × 10^{8} | (7) | |

Q_{i}^{G} | % | 98 ± 2 | 97.5 ± 2 | (6) | |

Q^{G} | % | 98 ± 2 | (6) |

Samples | Stage II | Stage III | ||
---|---|---|---|---|

A_{II,}μA | t_{II,}s | A_{III,}μA | t_{III,}s | |

MLG | 2.5 ± 0.15 | 0.25 ± 0.03 | 5.9 ± 0.1 | 5.1 ± 0.3 |

MLG–QD Hybrid structures | 4.4 ± 0.15 | 0.31 ± 0.02 | 11.1 ± 0.1 | 5.3 ± 0.2 |

^{1}The fitting parameters A

_{i}and t

_{i}are obtained with Equation (8).

© 2020 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Reznik, I.; Zlatov, A.; Baranov, M.; Zakoldaev, R.; Veniaminov, A.; Moshkalev, S.; Orlova, A.
Photophysical Properties of Multilayer Graphene–Quantum Dots Hybrid Structures. *Nanomaterials* **2020**, *10*, 714.
https://doi.org/10.3390/nano10040714

**AMA Style**

Reznik I, Zlatov A, Baranov M, Zakoldaev R, Veniaminov A, Moshkalev S, Orlova A.
Photophysical Properties of Multilayer Graphene–Quantum Dots Hybrid Structures. *Nanomaterials*. 2020; 10(4):714.
https://doi.org/10.3390/nano10040714

**Chicago/Turabian Style**

Reznik, Ivan, Andrey Zlatov, Mikhail Baranov, Roman Zakoldaev, Andrey Veniaminov, Stanislav Moshkalev, and Anna Orlova.
2020. "Photophysical Properties of Multilayer Graphene–Quantum Dots Hybrid Structures" *Nanomaterials* 10, no. 4: 714.
https://doi.org/10.3390/nano10040714